Biosynthesis of nanoparticles and silver nanoparticles ... Keat et al. Bioresour.Bioprocess. DOI...
Embed Size (px)
Transcript of Biosynthesis of nanoparticles and silver nanoparticles ... Keat et al. Bioresour.Bioprocess. DOI...
Keat et al. Bioresour. Bioprocess. (2015) 2:47 DOI 10.1186/s40643-015-0076-2
Biosynthesis of nanoparticles and silver nanoparticles Cheah Liang Keat1, Azila Aziz1, Ahmad M Eid1,3 and Nagib A. Elmarzugi1,2*
Abstract In this century, the development of nanotechnology is projected to be the establishment of a technological evo- lutionary of this modern era. Recently, nanotechnology is one of the most active subjects of substantial research in modern material sciences and hence metal nanoparticles have a great scientific interest because of their unique optoelectronic and physicochemical properties with applications in diverse areas such as electronics, catalysis, drug delivery, or sensing. Nanotechnology provides an understanding on fundamental properties of objects at the atomic, molecular, and supramolecular levels. Besides, nanotechnology also leads an alternative technological pathway for the exploration and revolution of biological entities, whereas biology provides role models and biosynthetic constitu- ents to nanotechnology. The findings of this review are important to provide an alternative for the green synthesis of silver nanoparticles. It showed more cost-effective and environmental friendly application as well as easier for large production, with relation to the properties of silver nanoparticles as antimicrobial, can be served well as an alterna- tive antiseptic agent in various fields. Typically, silver nanoparticles are smaller than 100 nm and consist of about 20–15,000 silver atoms. Due to the attractive physical and chemical properties of silver at the nanoscale, the devel- opment of silver nanoparticles is expanding in recent years and is nowadays significant for consumer and medical products.
Keywords: Bio-nanotechnology, Silver nanoparticles, Plant-mediated synthesis, Antimicrobial agent, Biosynthesis, Nanotechnology
© 2015 Keat et al. This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
Background In recent years, nanotechnology is an escalating field of modern research (Edhaya Naveena and Prakash 2013) involving in synthesis design, characterization, produc- tion, and application of structures, devices, and systems by controlling shape and size at the nanometer scale (Madhuri et al. 2012). Nanotechnology also involves syn- thesis of nanoparticles of size ranging from 1 to 100 nm (EU 2011; Adlakha-Hutcheon et al. 2009). Moreover, there is a new branch of nanotechnology existing, which is bio-nanotechnology that integrates principles of biol- ogy with physical and chemical procedures to generate nano-sized particles with specific functions (Kathiresan
et al. 2009; Qi and Wang 2004; Roduner 2006). The bio- based protocols for synthesis of nano-metals are both environmentally and economically green as they are based on green chemistry principles and are simple, relatively inexpensive, and easily scaled up for larger scale production (Mohanpuria et al. 2008; Iravani 2011; Prabhu and Poulose 2012). However, the chemical meth- ods available are often expensive, utilize lethal chemicals, and are comparatively complex. Hence, biosynthesis of nanoparticles using biological agents such as microbes or plant extracts has gained much attention in the area of nanotechnology in last few decades (Malik et al. 2014). Generally, there are three main steps involved in green synthesis method, i.e., reaction medium selection, bio- logical reducing agent selection, and selection of non- carcinogenic substances for stability of nanoparticles (El-Shishtawy et al. 2011). Yet, plant-mediated prepara- tion of nanoparticles can be advantageous over other bio- based synthesis because the procedure of maintaining
*Correspondence: [email protected]; [email protected] 1 Research and Innovation Department, Institute of Bioproduct Development, Universiti Teknologi Malaysia, 81310 UTM Johor Bahru, Johor, Malaysia Full list of author information is available at the end of the article
http://orcid.org/0000-0001-7108-8028 http://creativecommons.org/licenses/by/4.0/ http://crossmark.crossref.org/dialog/?doi=10.1186/s40643-015-0076-2&domain=pdf
Page 2 of 11Keat et al. Bioresour. Bioprocess. (2015) 2:47
cell cultures can be omitted and it is also suitable for large scale production under non-aseptic environments (Makarov et al. 2014).
Silver nanoparticles are well-known antimicrobial agents in surgically implanted catheters in order to reduce the infections caused during surgery (Oei et al. 2012) and are proposed to possess anti-fungal, anti-inflammatory, anti-angiogenic, and anti-permeability activities. Silver is also one of the main components in the various creams for healing wounds (Saikia et al. 2015). However, silver nanoparticles are now being introduced as an alternative antibacterial agent replacing silver ions. Both silver ions and silver nanoparticles have inhibitory and lethal effects on bacterial species such as Escherichia coli, Staphylococ- cus aureus, and even yeast. But, the formation of com- plexes for silver ions is limited and the effect of the silver ions somehow remains only for a short period (Méndez- Vilas 2011). Yet, this drawback has been resolved by the application of the intact silver nanoparticles which have greater antibacterial properties by promoting the syn- thesis of reactive oxygen species such as hydrogen per- oxide (Mohammed 2015). In addition to antibacterial activity of the silver nanoparticles, a complete disrup- tion of the bacterial membrane of Escherichia coli cells was observed after few minutes in contact with silver nanoparticles under TEM analysis (Raffin et al. 2008). The high efficiency of silver nanoparticles is mainly due to the availability of larger surface area to volume ratio for interactions, easing the penetration and disruption of nanoparticles into the bacterial cells, as compared to micro-sized silver ions (Durán et al. 2010).
Preparation of Nanoparticles Generally, nanomaterials can be fabricated through two main methods, i.e., “top-down” and “bottom-up” (Fig. 1)
approaches (Forough and Farhadi 2010). The top–down approach basically works with the material in its bulk form, and the size reduction to the nanoscale is then achieved by specialized ablations, e.g., lithography, ther- mal decomposition, laser ablation, mechanical milling, etching, and sputtering (Abou El-Nour et al. 2010). Alter- natively, the “bottom-up” approach is more preferable for the preparation of nanoparticles, where involving a homogeneous system wherein catalysts (e.g., reducing agent and enzymes) synthesize nanostructures that are controlled by catalyst properties, reaction media, and conditions (e.g., solvents, stabilizers, and temperature). For instance, chemical reduction method is the most common synthetic pathway for metal nanoparticles syn- thesis (Pal et al. 2011). In the case of silver nanoparticles, the chemical reduction method is carried out based on the reduction of aqueous silver nitrate in an appropri- ate operating medium using chemical reductants such as sodium citrate or branched polyethylenimine. In this way, negatively charged silver nanoparticles can be obtained from the process using sodium citrate acting as reductant, while positively charged silver nanoparti- cles can be synthesized from the reaction with branched polyethylenimine as reductant (Moghaddam 2010). Thus, the physiochemical properties, surface, and morphologi- cal characteristics of nanoparticles can possibly be con- trolled depending on the subsequent application through variation in precursor concentrations and reaction condi- tions (Mason et al. 2012).
Green synthesis of nanoparticles There are a variety of chemical and physical preparation methods available for the fabrication of nanoparticles including radiation, chemical precipitation, photochemi- cal methods, electrochemical, and Langmuir–Blodgett
Spinning, Pyrolysis, Sol-gel processes, Supercritical
fluid synthesis, Chemical vapor deposition
Green Synthesis (Plants, Algae,
Bacteria, Fungi, Yeasts & Actinomycetes)
Etching, Mechanical milling, Sputtering,
Laser ablation, Lithography, Thermal
Fig. 1 General types of synthesis of metal nanoparticles
Page 3 of 11Keat et al. Bioresour. Bioprocess. (2015) 2:47
techniques, but these methods are often extremely expensive and non-environmental friendly due to the use of toxic, combustible, and hazardous chemicals, which may pose potential environmental and biological risk and high energy requirement (Awwad et al. 2013). The drawbacks of low production rate, structural particle deformation, and inhibition of particle growth are also encountered in these nanoparticles synthesis. Currently, there is a growing need to develop sustainable prepara- tion of nanoparticles that get rid of using harmful organic chemical substances, since noble nanoparticles are widely applied to areas of human contact (Shams et al. 2013). To achieve the principle of green chemistry process, it leads to in search of green synthesis of nanoparticles which can be done by five methods as below:
Polysaccharide method By using polysaccharide method